Microstructure, mechanical property and in vitro ... length article Microstructure, mechanical...
Embed Size (px)
Transcript of Microstructure, mechanical property and in vitro ... length article Microstructure, mechanical...
Available online at www.sciencedirect.com
Journal of Magnesium and Alloys 2 (2014) 181e189www.elsevier.com/journals/journal-of-magnesium-and-alloys/2213-9567
Full length article
Microstructure, mechanical property and in vitro biocorrosion behavior ofsingle-phase biodegradable Mge1.5Zne0.6Zr alloy
Tao Li, Yong He, Hailong Zhang, Xitao Wang*
State Key Laboratory for Advanced Metals and Materials, University of Science and Technology Beijing, Beijing 100083, China
Received 5 May 2014; accepted 27 May 2014
Available online 30 June 2014
The microstructure, mechanical property, and in vitro biocorrosion behavior of as-cast single-phase biodegradable Mge1.5Zne0.6Zr alloywere investigated and compared with a commercial as-cast AZ91D alloy. The results show that the Mge1.5Zne0.6Zr alloy had a single-phasesolid solution structure, with an average grain size of 34.7 13.1 mm. The alloy exhibited ultimate tensile strength of 168 2.0 MPa, yieldstrength of 83 0.6 MPa, and elongation of 9.1 0.6%. Immersion tests and electrochemical measurements reveal that the alloy displayed lowerbiocorrosion rate and more uniform corrosion mode than AZ91D in Hank's solution. The elimination of intensive galvanic corrosion reactionsand the formation of a much more compact and uniform corrosion film mainly account for the better biocorrosion properties of theMge1.5Zne0.6Zr alloy than AZ91D.Copyright 2014, National Engineering Research Center for Magnesium Alloys of China, Chongqing University. Production and hosting byElsevier B.V.
Keywords: Magnesium alloys; Biomaterials; Single-phase; Microstructure; Corrosion; Biodegradable
Open access under CC BY-NC-ND license.
Recently, biodegradable magnesium based alloys areexperiencing a renaissance as potential choice for implantmaterials in bone and cardiovascular surgery due to theiroutstanding biocompatibility, biodegradability, and verysimilar mechanical properties compared with bone [1e5].Even though much attention has been paid to optimize theperformance of these materials [6e11], comparably high
* Corresponding author. Tel.: 86 10 82375280; fax: 86 10 62333447.E-mail address: email@example.com (X. Wang).
Peer review under responsibility of National Engineering Research Center for
Magnesium Alloys of China, Chongqing University.
Production and hosting by Elsevier
2213-9567/Copyright 2014, National Engineering Research Center for Magnesium Alloys of China, Cho
corrosion rate is still the biggest obstacle on the way to clinicalapplications . On the other hand, at present the demand forbiodegradable materials with better performance is so urgent,while studies are still not sufficient .
In early investigations, a large amount of alloying compo-nents were added to magnesium alloys such as AZ91 [14e16],ZK60 [17e19], WE43 [15,20,21], LAE442 [21e23], andMge20Zne1Ca , with an intention of enhancing themechanical properties. These alloys generally contain manyprecipitates. In the multiphase magnesium alloys, however,potentials of second phases are higher than that of a-Mgmatrix . So intensive galvanic corrosion reactions willoccur beside the second phases and many corrosion pits mayform, sometimes leading to the falling off of unattacked sec-ond phases from the alloy body. This will cause stress con-centration and the coming rapid reduction of mechanicalintegrity of implants during degradation. Huan et al. demonstrate that ZK30 possesses a better corrosion
ngqing University. Production and hosting by Elsevier B.V. Open access under CC BY-NC-ND license.
182 T. Li et al. / Journal of Magnesium and Alloys 2 (2014) 181e189
resistance than ZK60 and they accredit that to the lower Zncontent in ZK30, since there is less second-phase particles andthus less micro-galvanic cells in ZK30. Rad et al.  alsoconclude that dissolution rate of MgexCa alloy increasessignificantly with increasing Mg2Ca content, and corrosiondamage in specimens with lower Ca content is more moderateand uniform than with higher Ca content. Based on the aboveconsideration, a single-phase structure may inhibit the highcorrosion rate of magnesium alloys to some extent.
Another consideration for implant biomaterials is thebiocompatibility. Aluminum element is mostly added tomagnesium alloys such as AZ91, AZ31, and AE21 to achieveboth solid solution strengthening and precipitation strength-ening. However, aluminum is a risk factor for causing Alz-heimer's disease  and muscle fiber damage . Therefore,Al-free magnesium alloys are recommended for biodegradablematerials. In addition, investigations show that addition of rareearth elements can enhance the corrosion resistance of mag-nesium alloys [30e32]. Nevertheless, controversies are stillexist on the biological effects of those rare earth elements ,and this process can dramatically increase the production costof alloys.
As Al-free magnesium alloys, high-strength MgeZneZrseries are widely studied. Researchers generally add a highcontent of Zn with 3%e6%, e.g., ZK30 , Mge5Zne0.3Zr, and ZK60 [17e19], which results in many second-phaseprecipitates and thus inevitable galvanic corrosions. Accordingto the above consideration, we have developed a single-phaseMge1.5Zne0.6Zr alloy to avoid intensive galvanic corrosionreactions . The Mge1.5Zne0.6Zr alloy exhibits perfectcorrosion properties in 5% NaCl solution . As a potentialdegradable biomaterial, it is strongly needed to characterizethe biocorrosion behavior of the Mge1.5Zne0.6Zr alloy insimulated body fluid. In the present study, the microstructure,mechanical property and especially in vitro biocorrosionbehavior in Hank's solution of the as-cast single-phasebiodegradable Mge1.5Zne0.6Zr alloy are investigated andcompared with a commercial AZ91D alloy.
2.1. Sample preparation
Thealloywith the nominal compositionofMge1.5Zne0.6Zrwas prepared by the gravity casting process in a protective at-mosphere. The details can be referred to our former research. The actual chemical compositions were determined byinductively coupled plasma atomic emission spectroscopy (ICP-AES, Varian 715-ES, USA), as given in Table 1. To verify the
Chemical compositions of the as-cast Mge1.5Zne0.6Zr and AZ91D alloys
Alloy Al Zn Zr Fe Ni Cu Mg
Mge1.5Zne0.6Zr e 1.25 0.55 0.01 0.012 0.01 BalanceAZ91D 8.99 0.61 e 0.003 0.001 0.003 Balance
effectiveness of eliminating the galvanic corrosion of the single-phase magnesium alloy, a representative double-phase as-castAZ91Dalloy (BeijingGuangling JinghuaScience&TechnologyCo., China) was used as a reference. The AZ91D alloy is chosenbecause it is one of the most commonly used magnesium alloysand is believed to have good corrosion resistance . Also,AZ91D has been widely studied as a potential biodegradablematerial [14e16,36e38].
2.2. Microstructure characterization and mechanicalproperties evaluation
The microstructure of as-cast Mge1.5Zne0.6Zr andAZ91D alloys were observed using an optical microscope(OM) after prepared by a standard metallographic procedureand then followed by chemical etching in a solution of 12 gpicric acid, 80 ml acetic acid, 350 ml ethanol, and 80 ml water.The phase structure was detected by X-ray diffraction (XRD,Rigaku TTRIII, Japan), with a scan range from 10 to 100 and ascan speed of 8/min. The XRD measurements were operatedat 40 kV and 150 mA, using Cu Ka radiation.
Tensile tests were carried out on an MTS810 universaltesting machine at a constant crosshead speed of 1.0 mm/minat room temperature. For tensile tests, specimens were cut byan electric-sparking wire-cutting machine from the as-castalloys and machined to a gauge size of F6 mm 30 mm.Three specimens were tested for each alloy.
2.3. In vitro immersion tests
Immersion tests were conducted at 37 0.5 C in a Hank'ssolution, with a pH value of 7.4 adjusted with NaOH and HClsolutions. The Hank's solution was composed of 8.0 g/L NaCl,0.4 g/L KCl, 0.14 g/L CaCl2, 0.35 g/L NaHCO3, 1.0 g/Lglucose (C6H6O6), 0.1 g/L MgCl2$6H2O, 0.06 g/LMgSO4$7H2O, 0.06 g/L Na2HPO4$12H2O, and 0.06 g/LKH2PO4 in distilled water . For in vitro immersion tests,specimens with a gauge size of 10 mm 10 mm 3 mm werecut from the as-cast alloys. A hole of 1 mm in diameter wasdrilled near one edge of each sample to accommodate a nylonstring to suspend it in the solution during immersion test. Inorder for immersion test, the specimens were polished using2000 grit SiC papers. The solution volume to specimen surfacearea ratio was 30 ml/cm2 according to ASTM G31-72 .The test lasted for 168 h and the immersion solution wasrenewed every 24 h. After immersion test, the corrosionproducts were removed from the specimens in a chromic acidsolution of 200 g/L CrO3 and 10 g/L AgNO3 according toASTM G1-90 . The generation of hydrogen gas and thevariation of pH value in the Hank's solution were monitoredduring a continuous immersion test lasting for 168 h. Threespecimens were tested for each alloy at the same time. Thesurface morphologies of specimens before and after removingcorrosion products were examined by a field emission scan-ning electron microscope (FE-SEM, Zeiss Supra 55, Ger-many) equipped with a